UNCLASSIFIED MASTER COPY t FOR REPRODUCTION PURPOSFSECURITY CLASSIFICATION OF THIS PAGE
REPORT Ila. REPORT SECURITY CLASSIFICATION
Uncasi AD-A2302a. SECURITY CLASSIFICATION AUTHORITY A -AT82b. DECLASSIFICATIONiDOWNGRADING SCHEDUL- Approved for public release, A.ji
distribution unlimited.4. PERFORMING ORGANIZATION REPORT NUMBER(S) S. MONITORING ORGANIZATION REPORT NU ER(
6a. NAME OF PERFORMING ORGANIZATION 6b. OFFICE SYMBOL 7a. NAME OF MONITORING ORGANIZATION J(If applicable,
UNIVERSITY OF ILLINOIS U. S. Army Research Office
6c. ADDRESS (City, State, and ZIP Code) 7b. ADDRESS (City, State, and ZIP Code)
P. 0. Box 12211URBANA IL 61801 Research Triangle Park, NC 27709-2211
8a. NAME OF FUNDING /SPONSORING 8b. OFFICE SYMBOL 9. PROCUREMENT INSTRUMENT IDENTIFICATION NUMBERORGANIZATION (If applicable)
U. S. Army Research Office -Df:fIL.S0 3 6-k-O 018c. A, (RESS (City State. and ZIP Code) 10. SOURCE OF FUNDING NUMBERS
P. 0. Box 12211 PROGRAM PROJECT TASK WORK UNITELEMENT NO. NO. NO. ACCESSION NO
Re-:Pdrch Triangle Park, NC 27709-2211
11. TITLE (Include Security Classification)
STRENGTH OF POLYMER INTERFACES
12. PERSONAL AUTHOR(S)R. P. WOOL
13a. TYPE OF REPORT "13b. TIME COVERED 14. DATE OF REPORT (Year, Month, Day)111,5 PAGE COUNTFINAL I FROM 1/86 TO 1/89 I 90/11/25 I
1'6. SUPPLEMENTARY' NOTATION ..The view, opinions and/or findings contained in this report are those
of the authr($).and sh uld not be construed as an fficial Department of the Army position,
17. COSATI CODES 18. SUBJECT TERMS (Continue on reverse if necessary and identify by block number)
FIELD GROUP SUB-GROUP 1110 POLYMER WELDING, INTERFACE STRUCTURE, FRACTURE, FATIGUE,
LAMINATION, DIFFUSION r c.~wC~&La 1 ~19. ABSTRACT (Continue on reverse if necessary and identify by block numbe.)
"- Studies df strength development at polymer-polymer interfaces are examined and applicaticns towelding of simil~r and dissimilar polymers are considered. The fracture properties of the weld, namely,fracture stress, 6, fracture energy, GIc, fatigue crack propagation rate da/dN, and microscopic aspects ofthe deformation process are determined using compact tension, wedge cleavage, and double cantileverbeam healing experiments. The mechanical properties are related to the structure of the interface viamicroscopic deformation mechanisms involving disentanglement and bond rupture. The time dependentstructure of the welding interface is determined in terms of the molecular dynamics of the polymerchains, the chemical compatibility, and the fractal nature of diffuse interfaces. Several experimentalmethods are used to probe the weld structure and compare with theoretical scaling laws. Results aregiven for symmetric amorphous welds, incompatible and compatible asymmetric amorphous welds,incompatible semicrystalline and polymer-metal welds. The relevance of interface healing studies tothermal, friction, solvent and ultrasonic welds is discussed.
20. DISTRIBUTION /AVAILABILITY OF ABSTRACT 21, ABSTRACT SECURITY CLASSIFICATION
I]UNCLASSIFIEDAJNLIMITED 0 SAME AS RPT. - DTIC USERS Unclassified22a. NAME OF RESPONSIBLE INDIVIDUAL 122b. TELEPHONE (inciude Are. Code} Uc. OfFiCE SMBOL
RICHARD P. WOOL (217) 333-2468
DO FORM 1473,84 MAR 83 APR edition may be used until exhausted SECURITY CLASSIFICATION OF THIS PAGEAll other editions are obsolete UNCIASSIFTED
UNIS 9 TE
STRENGTH OF POLYMER INTERFACES
Richard P. Wool
Department of Materials Science and EngineeringUniversity of Illinois, 1304 W. Green St., Urbana, Illinois 61801
Final Report, Proposal No. 22966-MSArmy Research Office, Durham, NC
Studies of strength development at polymer-polymer interfaces are examined andapplications to welding of similar and dissimilar polymers are considered. The fractureproperties of the weld, namely, fracture stress, or, fracture energy, GIc, fatigue crackpropagation rate da/dN, and microscopic aspects of the deformation process aredetermined using compact tension, wedge cleavage, and double cantilever beam healingexperiments. The mechanical properties are related to the structure of the interface viamicroscopic deformation mechanisms involving disentanglement and bond rupture. Thetime dependent structure of the welding interface is determined in terms of the moleculardynamics of the polymer chains, the chemical compatibility, and the fractal nature ofdiffuse interfaces. Several experimental methods are used to probe the weld structure andcompare with theoretical scaling laws. Results are given for symmetric amorphous welds,incompatible and compatible asymmetric amorphous welds, incompatible semicrystallineand polymer-metal welds. The relevance of interface healing studies to thermal, friction,solvent and ultrasonic welds is discussed.
Avail and/orDist Speci a l
The joining or welding of polymers can be accomplished by several techniquesinvolving thermal welding, vibrational welding, friction welding, solvent welding, surfacechemical modification, ion beam surface modification, resonance heating and other moreexotic but less common techniques. In this Report we focus on polymer welding where themolecules near the surfaces become mobile and the weld strength develops by a combin-ation of surface rearrangement, wetting and diffusion. The molecular mobility can beinduced by heat from friction, (ultrasonic) vibration, impact, hot plates, solvents, etc.
In recent years, we have considered the problem of strength development at polymer-polymer interfaces in terms of the static and dynamic properties of random-coil chains (1-4). When two pieces of molten polymer are brought into contact, wetting or closemolecular contact (van der Waals) first occurs followed by interdiffusion of chain segmentsback and forth across the wetted interface. After a contact time, t, we inquire as to themechanical energy, G, required to separate the two pieces as a function of time, temper-ature, T, contact pressure, P, and molecular weight, M, of the linear random-coil chains,i.e.,
G = W(t, T, P, M) (1)where W is the welding function to be determined. Solutions to -his problem haveapplication to similar situations involving polymer-polymer interfaces. For example,processing of powder and pellet resin, internal weld lines of polymer melts during extrusionand injection molding, welding of surfaces, lamination of composites, coextrusion, andautohesion of uncured linear elastomers.
In this Report, we focus on problems of welding and autohesion with emphasis onsymmetric interfaces where the same amorphous polymer exists on both sides of theinterface. Consideration is also given to the important case of incompatible asymmetricamorphous and crystalline interfaces where strength develops between two immisciblepolymers. We begin by introducing the reptation model (5, 6) for diffusion at a symmetricinterface and determlne a molecular description of the interface structure as a function ofthe variables, t, T, P, and M. We then discuss models to relate the interface structure tothe mechanical properties via a set of microscopic deformation mechanisms. The latterinvolve disentanglement by chain pullout, bond rupture and connectivity between chains.The predictions for welding, tack and green strength are compared with experiments andtheories (7-11) of other investigators.
Molecular Dynamics of Random-Coil Chains
The motion of individual chains in amorphous bulk materials or concentrated solutionsof linear random-coil (Gaussian) chains has been modelled by the reptation theory of deGennes (5) and Edwards (6). In this model the chain is confined to a tube having a similarshape as the random-coil configuration of the chain. The tube represents topologicalconstraints to la: ral motion of monomers imposed by the neighboring chains via entangle-ments and predt ninantly restricts motion of the chain to that along the curvilinear lengthof the tube. Our use of this model is illustrated in Fig. 1. At t = 0, the chain (solid line) isin its initial tube indicated by the dashed lines. The chain exhibits Brownian motion backand forth in the tube and because the chain ends are free to move in any direction awayfrom the tube, the memory of the initial tube position in space is gradually lost as shown attimes t2 and t3. However, the chain being in a dense system is always in a new tube butonly parts of the chain, usually towards the center, retain memory of the initial tube for therelaxation time, Tr. The length of chain, 1(t), which "escapes" from the initial tube is also arandom-coil chain obeying Gaussian statistics and we call it the minor chain (2). As theminor chain increases in length we can represent its static dimensions by a "most probable"spherical envelope as shown in Fig. 1.
MINOR MINOR' CHAIN C
H A IN
DI -_ M 1. (3)The mean square monomer displacement of the minor chains:
= 1/2. (4)The mean square center-of-mass diffusion distance, < X 2cm >:
= 2Dt. (5)The center-of-mass self-diffusion coefficient, D:
D = M -2 (6)The reptation time, Tr:
Tr = M 3 (7)The fraction of chain remaining in the tube, F(t):
F(t) = 1 - 4/73/ 2 (t/Tr)1 / 2 , (8)where t < Tr.For t > Tr, F(t) can be well approximated by (5, 12),
F(t) :% 8/;r2e't/Tr. (9)
Equations 8 and 9 form the basis for describing the viscoelastic shear relaxationmodulus of the Doi-Edwards(12) constitut